A Constitutive Model for Circular and Square Cross-Section Concrete Conﬁned with Aramid FRP Laminates

: Fiber-reinforced polymer (FRP) has been used for seismic retroﬁtting and structural re-inforcement over recent decades. Numerous researchers have created stress–strain models based on experimental data to predict the mechanical properties of FRP-conﬁned concrete. In this study, circular and square cross-section specimens with different design concrete strength were prepared, and the compressive strength of the specimens conﬁned with different layers of aramid FRP (AFRP) were measured in compressive tests. A constitutive model was proposed to simulate the uniaxial compressive stress–strain relationship of the AFRP-conﬁned concrete, which was derived from the Mohr–Coulomb failure envelope theory, and the corresponding axial strain was determined from the regression analysis. The internal friction angle of the proposed constitutive model was determined for the cylindrical concrete specimens conﬁned with one and two layers of AFRP. The compressive strength of one and two layers of AFRP-conﬁned concrete specimens were used to obtain the parameters of the constitutive model; the absolute average error between experimental and predicted compressive strength was 7.01%. Then, the constitutive model was used to predict the strength of a three-layer AFRP-conﬁned concrete specimen, and the absolute average error was 4.95%. The cross-sectional shape coefﬁcient of the square concrete specimen was obtained analytically. Substituting the cross-sectional shape coefﬁcient into the proposed constitutive model, the average absolute error of the square cross-section concrete specimen was about 3.84%. The results indicated that the proposed constitutive model can predict the compressive strength of circular and square cross-section concrete specimens conﬁned with AFRP.


Introduction
The deterioration of concrete structures is usually the result of inadequate maintenance, especially in highly seismic regions.Natural disasters such as earthquakes, hurricanes, and tsunamis could destroy reinforced concrete (RC) structures; therefore, increasing the strength of RC structures in the most efficient way has become an important issue.The existing retrofitting methods include steel plate jackets and fiber-reinforced polymer (FRP) jackets.
The advantages of FRP include a high elastic modulus; corrosion, acid, and alkali resistance; high strength; and light weight.The compressive strength of concrete specimens could be enhanced when confined with FRP material, and the axial strain would increase as well [1][2][3][4][5].In the current practice, carbon-fiber-reinforced polymer (CFRP) was one of the most popular FRP materials for repairing and retrofitting RC structural members [6][7][8].
The experimental results from recent studies showed that the ultimate axial compressive strength and the corresponding strain were effectively improved when the low-strength concrete specimens were confined with carbon fiber composite materials [9][10][11].Zhang et al. (2023) explored the compressive strength properties of CFRP and GFRP confined geopolymer concrete.The results indicated that, due to the higher tensile strength and elastic modulus of CFRP, the restraining effects of CFRP were greater than those of GFRP [12].
Recently, aramid fiber has attracted more attention from many researchers in civil engineering because it has the characteristics of better corrosion resistance and higher specific strength, and its elongation is higher than that of carbon fiber.Some researchers used aramid FRP (AFRP) to wrap RC cylindrical members; the results showed that the load-bearing capacity of RC cylindrical members was improved by increasing the AFRP layers [13][14][15][16][17][18][19].Although the maximum tensile strength of aramid fiber was not as high as that of carbon fiber, the elongation was twice the latter, which could significantly improve the deformation and energy absorption of the concrete under loadings.The material properties of the commonly used fibers for FRP repair and retrofit are shown in Table 1 [20][21][22][23][24][25].For CFRP-confined concrete, the lateral confinement stress of CFRP was usually 15 to 30 times the lateral confinement stress of steel reinforcement (spiral); therefore, the axial compressive strength of the CFRP-confined concrete was also higher than that of steel reinforcement confined concrete.To estimate the peak uniaxial compressive strength of FRP-confined concrete accurately, a more effective and accurate formula must be established.In the last few decades, the constitutive models of confined concrete have been researched extensively.Mander et al. proposed a functional equation to present the stress-strain relationship and introduced the "effectiveness coefficient" of reinforced concrete specimens with circular, square, and rectangular cross-sections [26,27].Mirmiran and Shahawy (1997) proposed an equation to predict the peak strength of glass FRP (GFRP) confined concrete [28].Razvi and Saatcioglu (1998) proposed a constraint equation for high-strength concrete [29].Li's research proposed the constitutive models for normal-strength and low-strength cylindrical concrete confined with CFRP, which was adopted from the Mohr-Coulomb failure theory to predict the compressive strength of CFRP-confined concrete [30][31][32][33][34]. Wang et al. (2012) found that the CFRP-confined-squarecross-section column failed suddenly via CFRP rupture at the corner of the column, and a modified confinement pressure model was proposed which considered the influence of cross-section size, effective rupture strain of CFRP, as well as hoop reinforcement [35].Some studies presented the results of experimental studies on concrete cylinders confined with CFRP composites and proposed confinement models for cylindrical concrete members wrapped with FRP [36][37][38][39].Toufigh et al. (2019) investigated the mechanical properties of a polymer concrete beam/pile confined with CFRP.The result showed that the ductility and bending capacity were enhanced when CFRP sleeves were filled with polymer concrete [40].
Djafar-Henni and Kassoul (2018) measured the compressive stress-strain relationships of 81 concrete cylinders confined with AFRP wraps and compared them with the proposed model, which agrees with experimental curves of AFRP-confined concrete cylinders [41].Arabshahi et al. (2020) proposed a model using an evolutionary algorithm named multiexpression programming; the stress-strain model predicted the behavior of AFRP-confined concretes with good accuracy [42].In addition, due to the effect of the corner radius of FRP confined square concrete specimens, the constitutive model was different from the circular specimens when forecasting the actual situation.Li et al. (2019) tried to rebuild a well-established stress-strain model for the FRP confined square concrete specimens based on the circular ones [11].However, the stress-strain model of FRP confined square crosssection concrete specimens was not precise enough to match the experimental results [11,43].Diboune et al. (2022) proposed a model to predict the ultimate strength, ultimate strain, and axial stress-strain relationship of square and rectangular concrete columns confined with CFRP wraps.The proposed model provides good accuracy compared with the other existing models [44].
The majority of the prediction models from the references were developed using experimental regression.Consequently, this study aims to build a constitutive model for AFRP-confined concrete specimens with circular and square cross-sections based on the Mohr-Coulomb failure envelope theory.The experimental compressive stress-strain relationships of AFRP-confined concrete were used to obtain the parameters of the proposed constitutive model and then compared with other studies to illustrate the accuracy of the proposed constitutive model.

Materials and Fabrication of Test Specimens
This section introduces the materials used in the preparation of AFRP-confined concrete specimens, including the material characteristics of aramid sheets and epoxy resin.The proportions of cement, sand, and aggregates are also listed in this section.

Aramid Fiber
Aramid fiber is a high modulus, low density, high specific strength, and organic synthetic high-tech fiber with good abrasion resistance.The applications of aramid fiber include military equipment, automotive components, flame-resistant clothing, sports equipment, etc.Although the strength of aramid fiber was slightly lower than that of carbon fiber, its elongation was higher.The unidirectional aramid fiber fabric (Kevlar ® 29, DuPont, Richmond, VA, USA) was used in this study.The mechanical properties of aramid fiber were tested to the standards shown in Table 2.

Epoxy Resin
Epoxy resin has the characteristics of excellent moisture resistance and low shrinkage during curing, and it may improve the mechanical strength of the composite.In this study, the weight mixing ratio of epoxy resin and hardener was 2:1 to produce SB838 epoxy resin (Sam Bond Int'l Corp., Taiwan).

Concrete Specimen Preparations
Aggregate is the main component resisting compressive stress in concrete.In this study, the weight ratio of coarse aggregates (3/8 and 6/8 gravel) was 1:1.The fineness modulus (F.M.) of fine aggregates and coarse aggregates were 3.05 and 7.5, respectively; the fineness modulus of all aggregates was 5.42.The concrete specimens were prepared with different water to cement (w/c) ratios, and the mixing ratio of cement, sand, and aggregate in the concrete was 1:1.81:4.52.A total of 156 concrete specimens were tested in this study.The concrete specimens had different cross-sections: 120 cylindrical concrete specimens (Ø10 × 20 cm and Ø15 × 30 cm) with five different w/c ratios (0.50, 0.55, 0.60, 0.65, and 0.70) and 36 square cross-section concrete specimens (20 cm in height and 10 cm in width) with three different w/c ratios (0.50, 0.55, and 0.65).Each of the unconfined and confined (one to three layers) concrete specimens with different w/c ratios included three specimens.
The concrete specimens were wrapped with AFRP laminates by hand and layered-up on the 18th day of curing.The epoxy was applied to the surface of concrete specimens and cured at ambient temperature for several hours.The epoxy resin was applied to the surface of the specimen to adhere to and saturate the aramid fiber sheet.The aramid fiber was saturated in the epoxy resin by using a paintbrush, and the remaining epoxy was squeezed out by using a flat plastic scraper.The overlay length is more than 10 cm for each layer of the AFRP laminate confinement, as shown in Figure 1.Before applying the next layer of the AFRP laminate, it would take 24 h for the epoxy resin to cure, and then the above steps were repeated for the required number of layers.Finally, the AFRP-confined concrete with epoxy was cured for more than 7 days at ambient temperature.
study, the weight ratio of coarse aggregates (3/8″ and 6/8″ gravel) was 1:1.The fineness modulus (F.M.) of fine aggregates and coarse aggregates were 3.05 and 7.5, respectively the fineness modulus of all aggregates was 5.42.The concrete specimens were prepared with different water to cement (w/c) ratios, and the mixing ratio of cement, sand, and ag gregate in the concrete was 1:1.81:4.52.A total of 156 concrete specimens were tested in this study.The concrete specimens had different cross-sections: 120 cylindrical concrete specimens (Ø10 × 20 cm and Ø15 × 30 cm) with five different w/c ratios (0.50, 0.55, 0.60 0.65, and 0.70) and 36 square cross-section concrete specimens (20 cm in height and 10 cm in width) with three different w/c ratios (0.50, 0.55, and 0.65).Each of the unconfined and confined (one to three layers) concrete specimens with different w/c ratios included three specimens.
The concrete specimens were wrapped with AFRP laminates by hand and layered up on the 18th day of curing.The epoxy was applied to the surface of concrete specimens and cured at ambient temperature for several hours.The epoxy resin was applied to the surface of the specimen to adhere to and saturate the aramid fiber sheet.The aramid fiber was saturated in the epoxy resin by using a paintbrush, and the remaining epoxy was squeezed out by using a flat plastic scraper.The overlay length is more than 10 cm for each layer of the AFRP laminate confinement, as shown in Figure 1.Before applying the next layer of the AFRP laminate, it would take 24 h for the epoxy resin to cure, and then the above steps were repeated for the required number of layers.Finally, the AFRP-con fined concrete with epoxy was cured for more than 7 days at ambient temperature.

Compressive Test
The compressive strength of the circular (Ø10 × 20 cm and Ø15 × 30 cm) and square cross-section concrete specimens with and without AFRP confinement are presented and discussed in this section.The AFRP-laminate-confined concrete specimens were tested with the universal testing machine at the Department of Civil Engineering, National Tai pei University of Technology.As per the ASTM C39/C39M-01 standard [45], the loading rate of the actuator was 0.21 MPa/s.In addition, the loading process was stopped when the axial load was decreased to 70 percent of compressive strength.In the compressive test, a load cell (WF 17120, Wykeham Farrance, Milan, Italy) with a 500 kN capacity and strain gauges (KFGS-20-120-C1 L3M2R, KYOWA, Tokyo, Japan) were utilized.Addition ally, a data acquisition system (KL-10, Geomaster Group, Tianjin, China) was used to ob tain the force and strain information during compressive testing.

Unconfined Concrete Specimens (Benchmark)
In this subsection, the compressive test results of unconfined concrete specimens with five different designed strengths and three different cross-sections are listed in Table

Compressive Test
The compressive strength of the circular (Ø10 × 20 cm and Ø15 × 30 cm) and square cross-section concrete specimens with and without AFRP confinement are presented and discussed in this section.The AFRP-laminate-confined concrete specimens were tested with the universal testing machine at the Department of Civil Engineering, National Taipei University of Technology.As per the ASTM C39/C39M-01 standard [45], the loading rate of the actuator was 0.21 MPa/s.In addition, the loading process was stopped when the axial load was decreased to 70 percent of compressive strength.In the compressive test, a load cell (WF 17120, Wykeham Farrance, Milan, Italy) with a 500 kN capacity and strain gauges (KFGS-20-120-C1 L3M2R, KYOWA, Tokyo, Japan) were utilized.Additionally, a data acquisition system (KL-10, Geomaster Group, Tianjin, China) was used to obtain the force and strain information during compressive testing.

Unconfined Concrete Specimens (Benchmark)
In this subsection, the compressive test results of unconfined concrete specimens with five different designed strengths and three different cross-sections are listed in Table 3.Five different designed compressive strengths for the specimens were controlled with different w/c ratios with the compressive strength ranging from 20 MPa to 34 MPa.* C is the circular specimen, and the number afterwards is the cross-section diameter of the specimen; S is the square specimen, and the number afterwards is the cross-section width of the specimen; W is the water/cement ratio (w/c) of the specimen in %.For example, C10W50 is the specimen with the diameter of 10 cm and a water/cement ratio of 50%.

Confined Concrete Specimens Ø10 × 20
The compressive stress-strain relationships and ultimate lateral strains were measured for the Ø10 × 20 cm confined concrete specimens.Table 4 shows the compression test results for cylindrical concrete specimens with different w/c ratios and confined with different layers of AFRP.The AFRP-confined layers were increased from one to three layers, and then the compressive strength for five different w/c ratios (0.5, 0.55, 0.6, 0.65, and 0.7) were increased by 28~134%, 61~181%, 60~206%, 89~271%, 101~259%, respectively.The ultimate lateral strains are also shown in Table 4.The lateral strain was measured by using strain gauges; two strain gauges were mounted on the surface, one-third and two-thirds of the height for each cylindrical concrete specimen measured from the bottom.As the water-cement ratio increases, the compressive strength decreases; whereas, as the number of confinement layers increases, the compressive strength increases.The axial stress-strain relationships of the unconfined C10W50 and confined C10W50 with one to three layers of AFRP are shown in Figure 2a-d, respectively.The AFRP confinement improves the axial strain capacity of concrete significantly.
As the water-cement ratio increases, the compressive strength decreases; whereas, as the number of confinement layers increases, the compressive strength increases.The axial stress-strain relationships of the unconfined C10W50 and confined C10W50 with one to three layers of AFRP are shown in Figure 2a-d, respectively.The AFRP confinement improves the axial strain capacity of concrete significantly.

Confined Concrete Specimens Ø15 × 30
In this subsection, the compression test results and the failure mode of AFRP-confined concrete specimens are discussed.Table 5 shows the compression test result of cylindrical concrete specimens confined with one to three layers of AFRP.As shown in Table 5, the compressive strength increased with the increasing number of AFRP layers, and the increasing percentage for the five different w/c ratios (0.5, 0.55, 0.6, 0.65, and 0.7) were 26~99%, 32~116%, 36~128%, 42~157%, and 68~190%, respectively.The enhancement effect for Ø15 × 30 specimens was similar to that in Ø10 × 20 specimens, in which the AFRP confinement improved the compressive strength of the specimens with high w/c content better than for specimens with lower w/c content.However, the strength increasing percentage was lower compared with Ø10 × 20 specimens because the effective lateral confined stress (  ) of AFRP decreased with the increased diameter of the cylindrical concrete

Confined Concrete Specimens Ø15 × 30
In this subsection, the compression test results and the failure mode of AFRP-confined concrete specimens are discussed.Table 5 shows the compression test result of cylindrical concrete specimens confined with one to three layers of AFRP.As shown in Table 5, the compressive strength increased with the increasing number of AFRP layers, and the increasing percentage for the five different w/c ratios (0.5, 0.55, 0.6, 0.65, and 0.7) were 26~99%, 32~116%, 36~128%, 42~157%, and 68~190%, respectively.The enhancement effect for Ø15 × 30 specimens was similar to that in Ø10 × 20 specimens, in which the AFRP confinement improved the compressive strength of the specimens with high w/c content better than for specimens with lower w/c content.However, the strength increasing percentage was lower compared with Ø10 × 20 specimens because the effective lateral confined stress ( f l ) of AFRP decreased with the increased diameter of the cylindrical concrete specimens.The influence of both the effect of confinement (ranging from one to three layers of AFRP) and the diameter (Ø10 and Ø15) on the compressive performance of the concrete specimens is elucidated in Equations ( 3) and (4) in Section 4.1.Consequently, it is evident that concrete members with larger diameters require the incorporation of more layers of FRP confinement to achieve the same level of strength enhancement.The post-test photographs of confined and unconfined cylindrical concrete specimens after the uniaxial compressive test are shown in Figure 3. Figure 3a shows the shear failure of an unconfined cylindrical concrete specimen.Shearing failure with spalling appeared in the AFRP-confined concrete specimens as shown in Figure 3b-d.The shear with spalling failure was more pronounced when increasing the number of the AFRP layers.As seen from the test results, the deformation of the concrete specimen was not uniform, and the measured lateral strains exhibit variation.The post-test photographs of confined and unconfined cylindrical concrete specimens after the uniaxial compressive test are shown in Figure 3. Figure 3a shows the shear failure of an unconfined cylindrical concrete specimen.Shearing failure with spalling appeared in the AFRP-confined concrete specimens as shown in Figure 3b-d.The shear with spalling failure was more pronounced when increasing the number of the AFRP layers.As seen from the test results, the deformation of the concrete specimen was not uniform, and the measured lateral strains exhibit variation.

Confined Square Cross-Section Concrete Specimens
The axial stress-strain relationships of the square cross-section concrete specimens (S10W65) without and with AFRP confinement are shown in Figure 4a-d.The confined concrete attained brittle failure before the AFRP rupture, and the measured AFRP-confined strain was less than the strain obtained from the coupon axial test.The compressive strength of the square concrete specimen was enhanced with one to three layers of AFRP confinement from about 24% to 139%, as shown in Table 6.The experimental compressive results and lateral strain of AFRP-confined square concrete specimens are also listed in Table 6.
concrete attained brittle failure before the AFRP rupture, and the measured AFRP-confined strain was less than the strain obtained from the coupon axial test.The compressive strength of the square concrete specimen was enhanced with one to three layers of AFRP confinement from about 24% to 139%, as shown in Table 6.The experimental compressive results and lateral strain of AFRP-confined square concrete specimens are also listed in Table 6.As seen in Table 6, the compressive strength of AFRP-confined concrete specimens was enhanced by increasing the layers of AFRP.From the experimental results, it was observed that the enhancement effects for AFRP-confined square cross-section concrete specimens were not as good as for the cylindrical specimens.The square cross-section concrete specimens tend to produce more confining stress concentrated around the corners and less confining stress at the edges.Therefore, the confining stress was not uniform for the square cross-section specimens.As seen in Table 6, the compressive strength of AFRP-confined concrete specimens was enhanced by increasing the layers of AFRP.From the experimental results, it was observed that the enhancement effects for AFRP-confined square cross-section concrete specimens were not as good as for the cylindrical specimens.The square cross-section concrete specimens tend to produce more confining stress concentrated around the corners and less confining stress at the edges.Therefore, the confining stress was not uniform for the square cross-section specimens.
The failure photos of the unconfined and confined square cross-section concrete specimens are shown in Figure 5.It can be seen that the AFRP ruptured around the corners of the square cross-section concrete specimens, and this was most likely caused by the confining stresses of the square cross-section concrete specimens concentrating around the corners.

S10W65L1
34 The failure photos of the unconfined and confined square cross-section concrete specimens are shown in Figure 5.It can be seen that the AFRP ruptured around the corners of the square cross-section concrete specimens, and this was most likely caused by the confining stresses of the square cross-section concrete specimens concentrating around the corners.

Strain Energy
The strain energy (  ) was defined as the area of the stress-strain relationship curve multiplied by the volume of the specimen as follows.
where  is the number of compressive stress data recorded via the universal test machine;   and   are the compressive stress and strain of the concrete specimens at point i;  is the volume of the specimens.Figures 6 and 7 summarize the strain energy of the cylindrical concrete specimens (Ø10 × 20) and the square concrete specimens.Compared with the unconfined specimens, the strain energy increase percentages for one to three layers of AFRP-confined cylindrical specimens and square specimens were between 466% to 2185% and 314% to 1621%, respectively.It could be concluded that the AFRP confinement significantly enhanced the strain energy capacity of concrete specimens.

Strain Energy
The strain energy (E s ) was defined as the area of the stress-strain relationship curve multiplied by the volume of the specimen as follows.
where m is the number of compressive stress data recorded via the universal test machine; σ i and ε i are the compressive stress and strain of the concrete specimens at point i; V is the volume of the specimens.Figures 6 and 7 summarize the strain energy of the cylindrical concrete specimens (Ø10 × 20) and the square concrete specimens.Compared with the unconfined specimens, the strain energy increase percentages for one to three layers of AFRP-confined cylindrical specimens and square specimens were between 466% to 2185% and 314% to 1621%, respectively.It could be concluded that the AFRP confinement significantly enhanced the strain energy capacity of concrete specimens.

Constitutive Model for AFRP-Confined Concrete
The proposed constitutive model for confined concrete consists of the stress-strain relationship from the initial point to the compressive strength and corresponding strain; the compressive strength value was adopted from the Mohr-Coulomb failure criterion, and the corresponding strain was determined with regression analysis from the experimental data.

Constitutive Model for Compressive Strength of the Confined Concrete
The compressive strength of confined concrete was adopted from the Mohr-Coulomb failure criterion, and it is incorporated in the following equation:

Constitutive Model for AFRP-Confined Concrete
The proposed constitutive model for confined concrete consists of the stress-strain relationship from the initial point to the compressive strength and corresponding strain; the compressive strength value was adopted from the Mohr-Coulomb failure criterion, and the corresponding strain was determined with regression analysis from the experimental data.

Constitutive Model for Compressive Strength of the Confined Concrete
The compressive strength of confined concrete was adopted from the Mohr-Coulomb failure criterion, and it is incorporated in the following equation: where σ 1 is the uniaxial compressive strength of rock; σ 3 is the lateral confining stress; φ is the internal friction angle; and C 0 is the uniaxial compressive strength without lateral confinement.It was used as a constitutive model to predict the peak compressive strength of concrete confined with AFRP materials.The mechanical behavior of concrete specimens confined with the AFRP is similar to rocks confined with lateral water pressure.Therefore, the proposed constitutive model can be expressed as follows: where f cc is the compressive strength of the confined concrete; f c is the compressive strength of the unconfined concrete; φ is the internal friction angle of concrete; and f l is the effective lateral confining stress of AFRP, which could be described with the following equation: where n is the number of AFRP wrapping layers; t is the thickness of a single AFRP layer; E k f is the elastic modulus of AFRP; ε k f is the ultimate lateral strain of AFRP measured from the compressive test; k c is a cross-section shape factor; and D is the diameter of the specimen.In this study, the internal friction angle was a function of the compressive strength and was expressed as follows: Tables 4 and 5 show the measured lateral strains (ε k f ) of cylindrical specimens wrapped with different layers of AFRP laminates, and the maximum lateral strain was about 2.5%.The elastic modulus (E c f ) and thickness of one-layer AFRP (t) were obtained from Table 2.The lateral confining stress ( f l ) of AFRP could be determined by substituting the parameters ε k f , n, E c f , and t as shown in Equation ( 4).For one to three layers of AFRP-confined cylindrical specimens, the calculated effective lateral confined stresses for specimens with a diameter of 10 cm were 8.84, 17.69, and 26.53 MPa, and for specimens with a diameter of 15 cm were 5.90, 11.79, and 17.69 MPa, respectively.
In this study, the specimens confined with one and two layers of AFRP were used as control variables of the analysis and then used to predict the compressive strength of specimens confined with three layers of AFRP.From Equation ( 5), the A 0 and B 0 were determined from experimental data from the regression analysis, as shown in Tables 4 and 5; the values of A 0 and B 0 were 20 and 0.002, respectively.
The coefficient of determination (R 2 ) was used to assess the performance of the proposed constitutive models for AFRP-confined concrete specimens and is expressed as Equation ( 6).
where x and y are experimental compressive strength and proposed compressive strength from Equation (3); and x and y are the average of experimental compressive strength and proposed compressive strength, respectively.
Substituting the compressive strength of the unconfined concretes ( f c ), the effective lateral confining stress of AFRP ( f l ), and the internal friction angle (φ) into Equation (3), the compressive strength ( f cc ) of the proposed constitutive model can be obtained.The average absolute error was 7.01% as shown in Table 7, and the R 2 for the proposed constitutive model and the experimental compressive results was 0.86.

Constitutive Model for Axial STRAIN at the compressive Strength
As the axial stress of the cylindrical concrete reaches the compressive strength ( f cc ), the AFRP ruptures and cannot provide confinement stress.The axial strain of AFRPconfined concrete at the compressive strength is ε cc , as shown in Figure 8.Therefore, the ε cc could be obtained from regression analysis and is expressed as Equation (7).
Buildings 2023, 13, x FOR PEER REVIEW 13 of 23 The parabolic stress-strain relationship was adopted by some researchers [30,46], and it can be expressed as follows: Substituting the parameters   ′ and   ′ of C10W70 from Table 7 into Equation ( 8), the stress-strain relationship of C10W70 confined with one, two, and three layers of AFRP confinement can be obtained, as shown in Figure 9.As seen in Equation ( 7), the lateral confined stress ( f l ) varies with the measured lateral strain (ε k f on the AFRP, and it affects the axial strain ε cc of AFRP-confined concrete at the compressive strength).By substituting parameters φ, ε c , ε cc , f l , and f c into Equation ( 7), the parameter α = 2.57 was determined from the regression analysis.The experimental strain of cylindrical concrete specimens was not uniform.Therefore, the coefficient of determination (R 2 ) for strain between the proposed constitutive model and the experimental result was 0.74.
The parabolic stress-strain relationship was adopted by some researchers [30,46], and it can be expressed as follows: Substituting the parameters f cc and ε cc of C10W70 from Table 7 into Equation ( 8), the stress-strain relationship of C10W70 confined with one, two, and three layers of AFRP confinement can be obtained, as shown in Figure 9.The parabolic stress-strain relationship was adopted by some researchers [30,46], and it can be expressed as follows: Substituting the parameters   ′ and   ′ of C10W70 from Table 7 into Equation ( 8), the stress-strain relationship of C10W70 confined with one, two, and three layers of AFRP confinement can be obtained, as shown in Figure 9.

Shape Factor for Square Cross-Section
As the experiment results shown in Table 6, the effectiveness of AFRP confinement for square cross-section concrete specimens was reduced compared with cylindrical concrete specimens.Therefore, it is necessary to design a new parameter, cross-section shape factor (k c ), for square cross-section concrete specimens.The shape factor (k c ) of the square specimens was defined as the ratio of effective confinement area (A e ) and section area (A), and it could be expressed as Equation ( 9), as shown in Figure 10.
The section area (A) is related to the length (d) and the radius of the chamfer (R c ) and can be expressed as Equation (10), and the effective confinement area (A e ) can be expressed as Equation (11), where d is the length of the square section, R c is the radius of the chamfer, and θ is the intersect angle, as shown in Figure 10. ) Figure 10.The effective confinement area of square cross-section concrete specimens.

Verification of the Constitutive Model
In this subsection, the material and dimension parameters of three-layer AFRP-confined cylindrical concrete specimens were substituted in Equation ( 3).The compressive

Verification of the Constitutive Model
In this subsection, the material and dimension parameters of three-layer AFRPconfined cylindrical concrete specimens were substituted in Equation ( 3).The compressive strength of confined cylindrical concrete specimens predicted with the proposed constitutive model exhibit a good relationship with experimental results.Table 8 shows the predicted and experimental compressive strength of three-layer AFRP-confined cylindrical concrete specimens; the average absolute error was about 4.95%.Figure 11 shows the coefficient of determination (R 2 = 0.906) between the proposed constitutive model predictions and the experimental results for AFRP-confined cylindrical concrete specimens.The results indicated that the proposed constitutive model can accurately predict the compressive strength of cylindrical concrete specimens confined with AFRP.
concrete specimens; the average absolute error was about 4.95%.
Figure 11 shows the coefficient of determination ( 2 = 0.906) between the proposed constitutive model predictions and the experimental results for AFRP-confined cylindrical concrete specimens.The results indicated that the proposed constitutive model can accurately predict the compressive strength of cylindrical concrete specimens confined with AFRP.

Predictions of Compressive Strength for Square Cross-Section Specimens
The studies reveal that the enhancing effect of compressive strength obtained by increasing the FRP confined rectangular or square cross-section concrete specimens was not as good as the effect of cylindrical specimens.According to previous studies [47][48][49][50][51][52][53], the enhancing effect of FRP-confined square specimens was decreased with decreasing ratio of the radius of the chamfer to the length.
The relationship between average absolute error and k c is shown in Figure 12.The lowest absolute error was obtained when k c = 0.52, which is substituted in Equation ( 9) to determine the corresponding intersect angle (θ).

Predictions of Compressive Strength for Square Cross-Section Specimens
The studies reveal that the enhancing effect of compressive strength obtained by increasing the FRP confined rectangular or square cross-section concrete specimens was not as good as the effect of cylindrical specimens.According to previous studies [47][48][49][50][51][52][53], the enhancing effect of FRP-confined square specimens was decreased with decreasing ratio of the radius of the chamfer to the length.
The relationship between average absolute error and   is shown in Figure 12.The lowest absolute error was obtained when   = 0.52, which is substituted in Equation ( 9) to determine the corresponding intersect angle ().Substituting the parameters  = 10 cm,   = 2 cm, and   = 0.52 into Equations ( 9) and ( 11),  was obtained as 81°.The intersect angle of 81° was substituted into Equation ( 9), and then   could be expressed with Equation (12).
Substituting   into Equation ( 4), the effective lateral confined stresses for one to three layers of AFRP-confined square-section concrete specimens were 4.89 MPa, 9.78 MPa, and 14.67 MPa, respectively.Then, substituting the effective lateral confined stresses The accuracy of the proposed constitutive model was verified with five other researchers' experimental data, as shown in Table 10.The material parameters (E f n, t, and ε f ), dimension (d and R c ), and strength ( f c ) of the specimens were substituted into the proposed constitutive model.The average absolute errors were less than 6.38%.The proposed constitutive model can predict both the compressive strength of square concrete specimens confined with AFRP but also square-section concrete specimens confined with other types of FRP.[14,17,18,41,42].To verify the effectiveness of the proposed model, it is necessary to compare its performance with some models proposed by other researchers.The compressive strength of three layer KFRP confined cylindrical concrete specimens with dimensions of φ Ø 10 × 20 cm and Ø15 × 30 cm was tested and predicted.

Reference
Aspect Ratio (h/D) Model D. and K. [41] Any ratio W. and W. [14] Any ratio A. and G. [42] Any ratio V. and O. [17] 2 (305/152) Table 12 shows the error analysis of compressive strength predictions for cylindrical concrete specimens confined with three layers of KFRP.The average absolute errors of other prediction models by [14,17,18,41,42] were 156.97%, 24.34%, 25.15%, 35.53%, and 45.52%, respectively.The compressive strengths between experimental results and the predictions made with the proposed constitutive model in this study were closer than others, and the average absolute error was 4.61%.

Conclusions
This study presents a constitutive model for the compressive strength of AFRPconfined concrete specimens of different cross-sections.The following conclusions were drawn based on the experimental results and the proposed constitutive model.

1.
The experimental data of the specimens confined with one and two layers of AFRP were used to obtain the internal friction angle (φ).The average absolute error of compressive strength between the proposed constitutive model and experimental results was 7.01%, and the coefficient of determination (R 2 ) was 0.86;

Figure 7 .
Figure 7.The strain energy of square cross-section concrete specimens.

Figure 7 .
Figure 7.The strain energy of square cross-section concrete specimens.

Figure 8 .
Figure 8.The stress-strain relationships of the cylindrical concrete specimens confined with and without AFRP.

Figure 8 .
Figure 8.The stress-strain relationships of the cylindrical concrete specimens confined with and without AFRP.

Figure 8 .
Figure 8.The stress-strain relationships of the cylindrical concrete specimens confined with and without AFRP.

Figure 10 .
Figure 10.The effective confinement area of square cross-section concrete specimens.

Figure 11 .
Figure 11.The coefficient of determination (R 2 ) of the proposed and experimental compressive strength of AFRP-confined cylindrical concrete specimens.

Figure 11 .
Figure 11.The coefficient of determination (R 2 ) of the proposed and experimental compressive strength of AFRP-confined cylindrical concrete specimens.

Figure 12 .
Figure 12.The relationship between average absolute error and different   .

Figure 12 .
Figure 12.The relationship between average absolute error and different k c .

Table 1 .
Material properties of fibers.

Table 3 .
Average axial compressive strength of the unconfined concrete specimens.

Table 6 .
Experimental results for the AFRP-confined square specimens.

Table 7 .
Experimental and proposed constitutive model for compressive strength of the specimens confined with one and two layers of AFRP confinement.

Table 8 .
Experimental and proposed constitutive model compressive strength of the specimens confined with three layers of AFRP confinement.

Table 8 .
Experimental and proposed constitutive model compressive strength of the specimens confined with three layers of AFRP confinement.

Table 10 .
The compressive strength of square concrete specimens from other researchers' experimental data and the proposed constitutive model.

Table 11
lists the prediction models from recent researchers

Table 11 .
The prediction models from recent researchers.

Table 12 .
The compressive strength error analysis of other prediction models.